Advances in Precast Concrete Sandwich Panels toward
Energy Efficient Structural Buildings
Sani Mohammed Bida 1,2, Farah Nora Aznieta Abdul Aziz 1,*, Mohd Saleh Jaafar 1, Farzad Hejazi 1, Abu Bakar Nabilah 1
1 Housing Research Centre (HRC), Department of Civil Engineering, Universiti Putra Malaysia (UPM), 43400, Serdang, Selangor, Malaysia
2 Department of Civil Engineering, Federal Polytechnic Bida, PMB 55, Bida, Niger State, Nigeria
1 Affiliation 1,2; firstname.lastname@example.org 2 Affiliation 1; email@example.com 2 Affiliation 1; firstname.lastname@example.org 2 Affiliation 1; email@example.com 2 Affiliation 1; firstname.lastname@example.org
* Correspondence: email@example.com, firstname.lastname@example.org ; Tel.: +60-012-702-0786
Abstract: Precast concrete sandwich panels (PCSP) are energy efficient building system that are achieved through an insulation layer created between the concrete wythes. The insulation layer is usually of low bearing strength material making it more applicable for non-structural building systems. Hence, shear connectors are introduced to improve its structural capacity, which subsequently degrade it thermal performance by serving as thermal bridges across the panel. This article review researches of alternative materials and methods used to improve the thermal efficiency as well as reduced the strength loss due to insulation in PCSP. The alternative materials are basalt fiber reinforced polymer (BFRP), carbon fiber reinforced polymer (CFRP), glass fiber reinforced polymer (GFRP), and foam concrete which are selected due to their low thermal conductivity for use in shear connection. While thermal path method has been used to prevent the effect of thermal bridges. Although, some of these materials have successfully achieved the desirable behaviours, however, several undesirable properties such as brittleness, bond slip, the sudden crushing of the panel system, and FRP failure below its ultimate strength were observed. Hence, the practicality of the alternative materials are still questionable despite its higher cost compared to the conventional steel and concrete used in PCSP system.
Keywords: alternative materials, fibre reinforced polymer, insulation, precast concrete sandwich panel, shear connection, thermal efficiency.
Energy consumption in buildings is increasing due to human activities and global warming. The consumption is mostly as a result of thermal comfort due to electric heating and cooling requirements . Investigation has shown that energy invested in thermal comfort for buildings in Mediterranean areas is about 47.8% of the total annual energy consumed in Spanish homes . In Europe, about 30% of total energy is used for thermal comfort. Also, electric heating and cooling requirement for housing account for about 50–70% of energy used in America . On the average, buildings account for about 25–40% of total energy consumption which is mostly due to space heating or cooling requirements . Energy performance assessment of existing residential housing recorded an average thermal transmittance (U-value) of 1.77 W/m2K for wall panels . The thermal transmittance recorded above fall short of the maximum recommended U-value for near Zero Energy Buildings (nZEB) . This is
coming at the expence of the scarce resources and low economic status coupled with environment consequences.
Therefore, various governments’ agencies across the world have set targets in an effort to conserve the energy toward near zero energy buildings (ZEBs). This efforts are have made many countries to consider energy performance of building as a policy; in the Europe, EU Directive on Energy Performance of Buildings (EPBD) was set to the year 2020 in which all new buildings are expected to comply with “nearly zero energy buildings” . In the United States, US Department of Energy (DOE) unveiled its strategic master plan toward “marketable zero energy homes in the year 2020 and commercial zero energy buildings in 2025” [7, 8]. Similar policies have been enacted in many countries as shown in Table 1.
Table 1. Green and sustainable building initiatives across the world Country Green Building Program Year of
Initiation Achievement to date
Autralia Green Star 2003 1900 Green rated
projects Brazil Aqua/ LEED Brasil 2010 1,308 registered
projects Canada LEED canada/Green
Globes 2000 2576
China GBAS 2006 -
Finland PromisE 1998 -
France HQE 1996 16000
Germany DGNB 2007 2800 certificates
Hong Kong HKBEAM 2009 Over 1000
India Indian Green Building Council (IGBC)
2007 Over 4794 buildings
Indonesia Indonesian Green building Council (Greenship)
Italy Protocollo Itaca 2000 -
Japan CASBEE 2004 500 Over buildings
Korea KGBC 2000 1786
Malaysia Green Building Index
(GBI) 2008 Over 300 projects
Mexico LEED Mexico 2000 Over 94000
Netherlands BREEAM Netherlands - -
New Zealand Green Star NZ 2005 153 buildings
Portugal Lider A 2005
Singapore Green Mark 2005 Over 360 projects
South Africa Green Star SA 2007 -
United States Build it
Green/LEED/IGCC/ 1993 -
United Kingdom BREEAM 1990 -
Emirate Estidama 2009 -
Jordan EDAMA 2009 -
Therefore, the most sustainable way to reduce energy consumption for indoor thermal comfort is by controlling the exterior-interior thermal mass transfers through the envelope of the building components. This can be achieved through energy retrofitting of existing buildings and an innovative energy efficient approach to new constructions . According to Gervásio , energy sustainability in buildings is best achieved through material and energy efficiency. Hence, optimization of energy use such as in heating and cooling during building’s service period is best achieved by introducing an insulation material into the building. This has called for a renewed interest in energy conservation and efficiency in building components such as precast concrete sandwich panels (PCSP) system which uses insulation as thermal barrier.
2. Sandwich Systems
Generally, sandwich refers to the combination of different material together either in layers or as a matrix to form a composite. This approach can be implemented in various materials and systems depending on its intended application. Before 1960, the greatest breakthrough of sandwich system is in aerospace applications specifically in the development of Mosquito aircraft during the World War II. Post-1960, tremendous alternative uses of sandwich technology were witnessed in many areas such as automobiles, refrigeration facilities, ship buildings and building construction [10-12]. As building material, sandwich panels are used as precast components named Precast Concrete Sandwich Panel (PCSP). It is a modification of solid panels produced using industrialized building system (IBS) approach and have gained popularity in civil engineering applications due to its thermal performance [13, 14]. It offers better thermal efficiency than other traditional masonry construction or solid panel building methods due to the insulation material created between the concrete layers.
2.1. Precast Concrete Sandwich Panels
differ in mechanical properties and their thermal resistance depends on the type of insulation used. The choice of type of insulation in PCSP system does not only depend on thermal insulation capacity, but also on the combined performance based on different properties such as thermal conductivity, water absorption, permeability, and thermal expansion . Usually, low absorption insulation materials are used in other to minimize loss of water during production . However, in many building applications, expanded polystyrene (EPS) is the most used insulator in PCSP. The reasons are due to its low cost, low water absorption, low density, and availability in open market.
Figure 1: Section through precast concrete sandwich panel 
3. Research advances in precast concrete sandwich panels
Although, precast concrete sandwich panels (PSCP) offers better thermal efficiency than other solid wall building construction methods due to the insulation layer created between the concrete layers. However, the strength is sacrificed due to the inclusion of the insulation material to achieve a better thermal properties. Hence, the layers are connected by means of shear connectors through the insulation to improve the structural capacity and ensure composite action. Unfortunately, the connection that bind the individual layers together cause thermal bridges and are the main contributors to the thermal mass transfer from one side of the panel to the other [16, 22, 23]. Therefore, research advances in PCSP has taken two dimensions; the use of alternative materials for the fabrication of the panel components and design approach.
3.1. Materials Approach
A paradigm shift in the material used for the fabrication of the component parts of the PCSP system is witnessed from conventional concrete and steel to foamed concrete and fibre reinforced polymers (FRP) for wythes and shear connection, respectively in literature. Because, this materials are believed to exhibit lower thermal conductivity compared with the conventional materials.
3.1.1. Alternative Material for Wythes in PCSP
produce the highest conductivity values. Therefore, many researchers have attempted to improve the thermal performance of concrete wythes by developing lightweight concrete known as foamed or aerated concrete in PCSP production. In 2015, Amran  defined foamed concrete as a light cellular concrete produced from mixture of foaming agent in mortar which contains randomly distributed air voids and have a density range of 400–1850 kg/m3. It lower density makes it thermally more efficient than the conventional concrete. Also, foam concrete density of 1600 kg/m3 exhibits thermal conductivity of about 0.66 W/mK against 1.6 W/mK recorded for conventional concrete of density 2200 kg/m3 [26, 27]. Although, the low density of foamed concrete is also associated with low compressive strength which could impact negatively on the structural performance of PCSP.
Mohamad  reported that the compressive strength of the foamed concrete used in producing the panel wythes have a significant effect on the load capacity of the panel and premature crushing and buckling near the supports was observed when slenderness ratio above 18 was used. In addition, Mohamad and Muhammad  reported that premature material failure was observed when foamed concrete sandwich panel was tested under eccentric loading. It was inferred that the premature failure and local buckling was because of the lower compressive strength of the foamed concrete below 15 MPa. Also, full-scaled investigation of precast foamed concrete sandwich panel under axial loading with slenderness ratio between 14 to 20 indicated crushing behaviour both at the top and bottom of the panels [29, 30]. This indicates that panels produced using foamed concrete exhibit sudden crushing, unless large cross-section are used. Also, bond slip has been reported between the foamed concrete and the reinforcement due to the low frictional resistance between the two materials. In the other hand, Nooraini  reported that foamed concrete with a density range between 300 kg/m3 to 1600 kg/m3 exhibits thermal conductivity between 0.10W/mK to 0.66 W/mK. Also, Jones and McCarthy  revealed that the thermal conductivity of foam concrete ranges between 0.23 and 0.42 W/mK at dry densities of 1000 and 1200 kg/m3, respectively. The above mentioned conductivity values are far below conductivity of conventional concrete of 1.88 W/mK. Furthermore, Amran  reported that every 100 kg/m3 reduction in density of foamed concrete lead to corresponding increase in thermal insulation by about 0.04 W/mK of the total thermal insulation. However, the reduction in density becomes a disadvantage in terms of structural efficiency. It exhibits high porosity and water absorption behaviour coupled with low compressive strength. The above mentioned criterion are not suitable for load bearing external walls which are subjected to climatic conditions such as rain and snow load, making it highly susceptible to water absorption.
Ideally, PCSP should be made from material of low water absorption. Unfortunately, foamed concrete have high porosity and permeability which is described as a measure flow of water under pressure in a saturated porous medium . It absorbs water twice as much as that of convention concrete at similar water cement ratio [33, 34]. Kearsley and Wainwright  reported that increase in cement ratio in foam concrete mixes increased the water vapour permeability proportionally most especially at the lower densities. Kochhar and Manohar  reported that moisture content is one of the major factors affecting the thermal conductivity of materials. The higher the material moisture content, the higher the thermal conductivity. Larson and Benner  also reported that thermal effectiveness of materials at a higher moisture content is reduced. Therefore, higher thermal conductivity values are recorded due to increased energy transfer by conduction and evaporation– condensation due to moisture transfer from warm to cold sides of the system. Moisture penetration into building materials could impact negatively on it thermal performance by increasing its thermal conductivity.
Therefore, wythes of a load bearing panels should be made from material of low water absorption without compromising its structural integrity. This feature could be achieved only if the strength of the panel is not affected or lowered. structural panel could be produced by increasing the thickness of the insulation layer while at the same time improve the shear connection design. By so doing, the strength loss due to insulation thickness could be augmented and the thermal performance improved.
3.1.2. Alternative Material for Shear Connection in PCSP
In order to reduce the effects of thermal mass transfer in PCSP, many research works have taken the option of using alternative materials that have low thermal conductivity such as carbon fibre reinforced polymer (CFRP) [39-41], Basalt fibre reinforced polymer (BFRP) [23, 42, 43], and Glass fibre reinforced polymer (GFRP) [44-51]. Theoretically, the structural behaviour and thermal performance of fibre reinforced polymers depends on their chemical composition.
According to Choi , it is difficult to predict the level of composite action, moment capacity and thermal deflections of FRP shear connector in PCSP, because of the variability in the chemical composition of the materials used in making the FRP. Besides, the material tends to exhibit many disadvantages particularly when used for structural applications. Naito  investigated the structural deformation behaviour of various configurations of FRP and steel shear ties in PCSP. It was observed that the FRP ties are stiffer than the steel ties. The latter produced a flexible response, coupled with large ductility. Furthermore, FRP materials are more expensive than the conventional steel material and the protrusion process during manufacturing of the FRP bars requires high-cost specialized machinery making it uneconomical for the proposed application . Some other disadvantages such as bond-slip, brittleness, low failure strain, low modulus of elasticity, delamination under loading and brittle failure without clear warnings are also reported when FRP materials are used in PCSP system [45, 54-56].
In 2014, Tomlinson and Fam  investigated the effect of GFRP in the precast concrete sandwich panel by sand coating the GFRP material to reduce bond slip. No pull-out failure was observed due to the sand coating, however, all the GFRP connectors were observed to fracture during the tests. The fracture is the result of the brittleness of the GFRP material when compared with conventional steel that is a ductile material. Earlier, Woltman  reported that the shear strengths of GFRP shear connectors are significantly lower than the values specified by manufacturer when tested in panels. This is because the connectors are usually tested under tension rather than direct shear. When used in the panel system where it is subjected to direct shear, the GFRP connectors failed in strength far below it stated strength by the manufacturer.
Jiang  carried out a direct shear push-out test to assess the performance of Precast Concrete Sandwich Panel (PCSP) with W-shaped Glass Fibre-reinforced Polymer shear connectors. The results indicate an elastic-brittle response caused by the pull-out of the connectors before the ultimate strength was reached. This indicates that the SGFRP material did not exhibit ductility behaviour. Many investigations have been carried out on the structural performance of PCSP with the alternative materials as summarized in Table 2(a)-(c). Despite the numerous investigations in this regard available in literature, no corresponding report yet regarding the thermal performance of the PCSP assemblies [40, 57]. Even though, report have shown that there is opposite behavior between the load capacity and thermal efficiency: increasing number of shear connectors increases the load capacity, but decreases thermal performance. However, Salmon  reported that the thermal conductivity of CFRP material is about 14% of steel conductivity, which encourages more research in using FRP as shear connector in PCSP system.
respectively as against the foamed concrete which recorded the ultimate load of 890 kN coupled with higher early crack range of 63-94%. In 1997, Salmon et al. introduced the use of FRP as shear connection material and since then, most attention have been drifted toward the use of the material for shear connection. Ultimate flexural load of 117.3 kN was achieved by using conventional steel and concrete while the range of 4-95 kN has been recorded for FRP. Even though, the upper limit were obtained from the control samples that are made up of the conventional concrete and steel. Table 2(c) shows the shear behaviour of precast concrete sandwich panels. The range between 5-138 kN/m was recorded mostly from the use of FRP for shear connection. The highest value of 138 was achieved due to the larger embedment length and the corrugation of the FRP shear connectors used in the specimen. The increase in the embedment length leads to increase in the cross sectional area of the sample, making it uneconomical for commercial application.
Table 2(a). Summary of previous works on PCSPs under Axial Loading
Material Shear Connection Material
Material Ultimate Load (kN)
First crack (%)
Amran  Foamed
Concrete steel EPS 250-850 33–82 Rahman and Jaini
 Foamed Concrete steel truss - 280-441 - Mohamad and
Hassan  Foamed Concrete steel EPS 355-890 34-64 Carbonari  Concrete steel EPS 102-666 -
Gara  Concrete steel EPS 400-500 -
Mohamad  Foamed
Concrete steel EPS 250-600 51-72 Mohamad and
Muhammad  Foamed Concrete steel truss EPS 188-355 63-94 Benayoune  Concrete steel polystyrene
foam 1250-1450 44–79
Benayoune  Concrete steel EPS 1051 38-55
Farah  Concrete steel EPS 595-930 -
Table 2(b). Summary of previous works on PCSPs under Flexural Loading
Material Shear Connection Material
Material Ultimate Load (kN)
First crack (%)
Amran  Foamed
Concrete Steel EPS 31-40 40-51
Kang and Kim  - GFRP EPS, XPS and
VIP - -
Kim and Choi  Concrete GFRP XPS foam 10-87 30-78 Kim and You  Concrete GFRP EPS, XPS
Tomlinson and Fam  Concrete BFRP EPS 38-41 -
Tomlinson and Fam  Concrete GFRP &
concrete Rigid foam 17-95 32-83
Sousa  Concrete GFRP XPS 60-70 -
Mathieson and Fam  GFRP skin GFRP polyurethane 7-28 -
Henin  Concrete GFRP XPS 44-90 -
Flores-Johnson and Li
 Foamed Concrete, FRFC
Steel encased concrete
- 18-44 -
Gara  Concrete Steel EPS 13-20
Frankl  Concrete CFRP XPS, EPS 45-90 -
Pantelides  Concrete GFRP EPS 25-45 -
Lee and Pessiki  Concrete Steel - 30-36 20-52 Benayoune  Concrete steel polystyrene
foam 117.3 55–60
Lee and Pessiki  Concrete steel - - -
Salmon  Concrete FRP - 4.4-22 -
Bush and Stine  Concrete steel EPS 14-21 -
Table 2(c). Summary of previous works on PCSPs under Shear Loading
Material Shear Connection Material
Material Ultimate Load (kN/m)
First crack (%)
Tomlinson  Concrete BFRP EPS 42808 -
Kazem  Concrete CFRP and GFRP EPS, XPS
foam 30-105 -
Choi  Concrete GFRP EPS, XPS 49-138 -
Hodicky  Concrete CFRP EPS 25-90 -
Woltman  Concrete GFRP XPS 21-78 -
Oh  Concrete GFRP EPS and XPS 19-51 -
Sousa  FRP GFRP XPS 60-70 -
Soriano and Rizkalla
 Concrete GFRP and CFRP EPS, XPS 59-129 -
Naito  - BFRP, CFRP,
GFRP & solid concrete
EPS, XPS 5 - 18 -
Cho  Concrete FRP FRP - -
EPS-expanded polystyrene, XPS-extruded polystyrene, CFRP- carbon fibre reinforced polymer
3.1.3. Insulation Materials
polystyrene, polyurethane board, blanket batt, rock wool, loose fill perlite, rigid form, reflective form, roll form, loose-fill form, foamed in place and glass fibre. The choice of insulation type depends on it intended application, thermal insulation capacity, water absorption behaviour and other thermal and physical properties required. The thermal conductivity of these materials are within the range of 0.026-0.05 (W/mK) depends on their densities. However, polystyrene offer better advantages of lower water absorption, high thermal insulation, and lightweight and above all does not release poisonous gases when ignited. Moreover, polystyrene products show least sensitivity to changes in temperature and are easy to handle (can be cut to size and adjusted) during installation . This is more reason why more of polystyrenes are being used in precast concrete sandwich panels than other insulation materials.
Selection of appropriate insulation location in sandwich panels through optimization of location and thickness of the insulation material plays a vital role in reducing energy consumption by restraining heat transmission loads to and from the buildings and would consequently reduce the demand for air-conditioning or heating. Many research works have been carried out to investigate the appropriate location and thickness of the insulation materials for best performance. In 2006, Bolattürk  reported the minimum and maximum insulation thicknesses using polystyrene insulation material to be in the range 20 to 170 mm with about 22 to 79% energy savings. Ucar and Balo  investigated the optimum insulation thickness of wall system in four climate regions of Turkey, by using foamboard 1500, foamboard 3500 fiberglass and extruded polystyrene as insulation materials. However, it was recommended that the optimum insulation thickness between 10.6 to 76.4 mm should be used for best performance.
For a structural panels, the requirement for symmetry in the sizes of the two wythes is of paramount importance to sustain the load capacity and compositeness of the sandwich system. This can be ensured when the insulation is placed at the middle of the panel. This approach is consistent with the findings by Kossecka and Kosny  who reported that thermal performance of walls depend significantly on the type of climate, either hot or cold and it best performance is achieved by locating the insulating layer at the inner core of the walls. In 2011, Ozel  investigated thermal performance of extruded polystyrene (XPS) and expanded polystyrene (EPS) insulation materials based on optimum insulation thickness of building walls with different structure materials under dynamic thermal conditions. The result show that the optimum thickness of insulation material varies between 20 to 82 mm. In 2012, Ekici  investigated the insulation thickness of expanded polystyrene, extruded polystyrene, Fiberglass, and foamed polyurethane materials in various wall assemblies. The result showed that an insulation thickness in the range of 20 and 186 mm is appropriate for best performance.
Yu  reported that selection and determination of appropriate insulation material and thickness is of paramount importance in reinforced concrete sandwich system and that expanded polystyrene proved to be the most efficient insulation material when compared with extruded polystyrene, foamed polyurethane, perlite and foamed polyvinyl chloride in terms of overall performance and cost and recommended between 53 to 236 mm as thickness of the insulation material. The thermal efficiency of a wall assembly system depends on the type of insulation, thickness, and density of the insulation material. Computing the total thermal resistance of a multi-layered wall assembly would require summation of all the resistances of the individual layers . The performance of the insulation resistance in the assembly system to heat flow would depend on how and where the insulation is installed. Location of insulation layer in a single layered wall panel is immaterial and when multi-layered insulation is used, the sum of the thickness of all the layers is the same as the optimum thickness in the single layered panel .
insulation of equal thickness at outer and inner sides of the wall assembly yield the best performance in terms of thermal efficiency. This claim was also supported by Al-Sanea and Zedan .
Summarily, it could be deduce from the above reviews that the best insulation location is when the insulator is located at the middle or the exterior part of the panel assembly. However, the middle core provides a symmetrical behaviour for best composite action for structural applications. Also, the most effective thickness for insulation material in term of thermal resistance is 10.6-186 mm depending on the type of insulator. However, polystyrene have been recommended as the best when considering overall performance.
3.2. Design Approach
The main aim of designing precast concrete sandwich panel is to develop a thermally efficient panel. This aim could be achieved either through the use of alternative material or design method. The alternative materials approach as discussed above indicated promising prospect for used in PCSP. However, its application comes with many challenges such as bond slip, brittleness, low structural strength and uneconomical section. Therefore, innovative design approach could offer more economical and thermally efficient structural panels.
In 1987, Zarr  introduced a sandwich panel referred to as super-insulated wall panel by using thermal path approach. The panels were designed using timber material which are staggered in framing to increase thermal flow path and break direct thermal bridges between the two sides of the panels. The thermal insulation capacity of the super-insulated timber panels were observed to be three times that of the conventional wood panel. Similar concept was implemented in three-layer PCSP with a total thickness of 279.4 mm by Lee and Pessiki . The panels indicated improved thermal performance by 19.8% compared with the control specimen of direct connection. However, the authors reported that the panel is un-economical due to its excessive thickness and required cumbersome production method leading to prolonged production time. Also, the excessive concrete volume leads to increase weight and cost of materials. In an attempt to improve the challenges aforementioned, the thermal path concept was adopted in a 150 mm thick two-layer super-insulated precast concrete structural sandwich panels (SIPCSSP) by Bida . Three different staggered spacing of shear connectors were tested using hot box test method and verified by FEM model. Despite the conventional steel and concrete used in the panels, the results show improved thermal performance by 117% for 200 mm spacing, 207% for 300 mm spacing and 236% for 400 mm spacing as compared to the direct 200 mm shear connector spacing (control specimen). The results are well within the allowable near zero energy buildings (nZEB) requirements for new and sustainable buildings.
The thermal path approach implemented in PCSP using conventional materials is a design method that have demonstrated excellent thermal performance. At the same time, the challenges of brittleness, bond-slip and other related issues aforementioned in the use of alternative materials have been avoided. Therefore, more attention is needed to investigate structural performance of PCSP using the thermal path approach. The success of this approach could fast track compliance to the new trend of achieving the targets of near-Zero Energy Buildings enacted in many countries.
This paper presents a review of works carried out in the area of reinforced concrete sandwich panel system. It is observed that the research direction in this area has been concentrated on finding the most efficient panel system using alternative materials such as FRPs and foam concrete due to the high thermal conductivity of steel and conventional concrete. For a non-structural application, the existing system using alternative material is sufficient for use, since it requires only minimum shear connection. However, for structural application, better composite behaviour is required coupled with minimum thermal bridges.
be given careful attention especially for structural applications. However, current alternative materials used in the PCSP system comes with many undesirable disadvantages for use in structural applications such as bond slip, brittleness, low shear strength and un-economical sections. The alternative materials in PCSP for use in structural applications are expected to exhibit ductile behavior as obtainable in steel to ensure sufficient avenue for warning and evacuation in the event of failure coupled with low thermal conductivity. These features are yet to be achieved from the alternative material such as BFRP, CFRP, GFRP and foamed concrete in reinforced concrete sandwich panels. Thus, more investigations are required in this regard using a conventional material such as steel reinforcement and concrete to develop more design methods like thermal path approach rather than alternative materials that seem unsustainable for practical application in load bearing systems. However, to achieved better and more efficient PCSP using FRP materials, a ductile and slip resistant materials are required to satisfy both the thermal and structural requirements.
Author Contributions: S.M.B and F.N.A. conceived the idea, wrote and analyzed the review; M.S.J, F.H and A.N updated and edited the paper. All authors have read and approved this review.
Funding: The authors would like to acknowledge the fund provider for making this research a reality by paying for all the materials, fabrication and experimental tests through research grant 06-01-04-SF2364, Ministry of Science and Technology Malaysia (MOSTI).
Acknowledgments: The authors would like to acknowledge the contribution of the technicians and other individuals who contributed toward the success of this research.
Conflicts of Interest: The authors declare no conflicts of interest.
 Ryan, E.M.; Sanquist T.F. Validation of building energy modeling tools under idealized and realistic
conditions. Energ Buildings. 2012, 47
 Domínguez, S.; Sendra J.; León A.; Esquivias P. Towards energy demand reduction in social housing
buildings: Envelope system optimization strategies. Energies, 5 (7): 2263-2287. 2012.
 Al-Homoud, M.S. Performance characteristics and practical applications of common building thermal
insulation materials. Building and environment. 2005, 40(3)
 Robinson, A.; Lesage F.; Reilly A.; McGranaghan G.; Byrne G.; O’Hegarty R.; Kinnane O. A new
transient method for determining thermal properties of wall sections. Energ Buildings. 2017, 142
 EU nZEB. Report on Nearly zero-energy buildings. 2012 June 22, 2017]; Available from:
https://ec.europa.eu/energy/en/topics/energy-efficiency/buildings/nearly-zero-energy-buildings.  Sartori, I.; Napolitano A.; Voss K. Net zero energy buildings: A consistent definition framework.
Energ Buildings. 2012, 48
 Chua, S.C.; Oh T.H. Green progress and prospect in Malaysia. Renew Sust Energ Rev. 2011, 15(6)
 Sood, S.M.; Chua K.; Peng D.L.Y. Sustainable development in the building sector: green building framework in Malaysia. ST-8: Best Practices & SD in Construction. 2011
 Gervásio, H.; Santos P.; da Silva L.S.; Lopes A. Influence of thermal insulation on the energy balance
 Mohamad, N.; Omar W.; Abdullah R. Precast Lightweight Foamed Concrete Sandwich Panel (PLFP) tested under axial load: preliminary results. Advanced Materials Research. Trans Tech Publ; 2011.  PCI Handbook. PCI design handbook: precast and prestressed concrete. 2007, MNL-120. 6th ed.
Chicago, IL: PCI.
 Davies, M. Wall transient heat flow using time-domain analysis. Building and Environment. 1997,
 Bai, F.; Davidson J.S. Analysis of partially composite foam insulated concrete sandwich structures.
Eng Struct. 2015, 91
 Benayoune, A.; Samad A.A.A.; Trikha D.; Ali A.A.A.; Ashrabov A. Structural behaviour of
eccentrically loaded precast sandwich panels. Constr Build Mater. 2006, 20(9)
 Bida, S.M.; Aziz F.; Jaafar M.S.; Hejazi F.; Nabilah A.B. Efficient Structural Sandwich Wall Panels
Devoid of Thermal Bridges, in Global Civil Engineering Conference (GCEC, 2017)Springer
 Kim, Y.J.; Allard A. Thermal response of precast concrete sandwich walls with various steel connectors for architectural buildings in cold regions. Energ Buildings. 2014, 80
 Benayoune, A.; Samad A.A.; Ali A.A.; Trikha D. Response of pre-cast reinforced composite sandwich
panels to axial loading. Constr Build Mater. 2007, 21(3)
 Pessiki, S.; Mlynarczyk A. Experimental evaluation of the composite behavior of precast concrete sandwich wall panels. PCI J. 2003, 48(2)
 Soriano, J.; Rizkalla S. Use of FRP grid for the composite action of concrete sandwich panels. Proceedings of the 11th International Symposium on Fiber Reinforced Polymer for Reinforced Concrete Structures (FRPRCS11), Guimarães, Portugal. 2013.
 Einea, A.; Salmon D.; Fogarasi G.; Culp T.; Tadros M. State of-the-art of precast sandwich panel system. PCI J. 1991, 36(6)
 Hamed, E. Modeling, Analysis, and Behavior of Load-Carrying Precast Concrete Sandwich Panels. J
Struct Eng. 2016, 142(7)
 Lee, B.-J.; Pessiki S. Thermal Behavior of Precast Prestressed Concrete Three-Wythe Sandwich Wall
Panels, in Building Integration Solutions
 Tomlinson, D.G.; Teixeira N.; Fam A. New shear connector design for insulated concrete sandwich
panels using basalt fiber-reinforced polymer bars. J Compos Constr. 2016, 20(4)
,04016003.  Hata, R.M.; Hassan R.; Idayu H.; Arshad F. The thermal conductivity of selected tropical timber
species using hot box method. Jurnal Teknologi. 2016, 78(5-4)
 Amran, Y.M.; Farzadnia N.; Ali A.A. Properties and applications of foamed concrete; a review. Constr
Build Mater. 2015, 101
 Mohd Zahari, N.; Abdul Rahman I.; Zaidi A.; Mujahid A. Foamed concrete: potential application in
thermal insulation. 2009.
 Nooraini, M.Z.; Ismail A.R.; Mujahid A.; Zahidi A. Foamed concrete: potential application in thermal
 Mohamad, N.; Muhammad H.M. Testing of precast lightweight foamed concrete sandwich panel with
single and double symmetrical shear truss connectors under eccentric loading. Advanced Materials Research. Trans Tech Publ; 2011.
 Amran, Y.M.; Rashid R.S.; Hejazi F.; Safiee N.A.; Ali A.A. Structural behavior of laterally loaded
 Amran, Y.M.; Rashid R.S.; Hejazi F.; Ali A.A.; Safiee N.A.; Bida S.M. Structural Performance of
Precast Foamed Concrete Sandwich Panel Subjected to Axial Load. KSCE J Civ Eng. 2018, 22(4)
 Jones, M.; McCarthy A. Heat of hydration in foamed concrete: Effect of mix constituents and plastic
density. Cement and concrete research. 2006, 36(6)
 Sabir, B.; Wild S.; O'farrell M. A water sorptivity test for martar and concrete. Materials and Structures. 1998, 31(8)
 Kearsley, E.P. The effect of high volumes of ungraded fly ash on the properties of foamed concrete.
1999, University of Leeds.
 Kearsley, E.; Wainwright P. Porosity and permeability of foamed concrete. Cement and concrete research. 2001, 31(5)
 Kochhar, G.S.; Manohar K. Effect of moisture on thermal conductivity of fibers biological insulating
materials. Thermal Performance of the Exterior Envelopes of Building VI. ASHRAE/DOE Conference. 1995.
 Larson, D.; Benner S. Field and laboratory studies of the thermal resistance of moist building insulation systems. Thermal Performance of the Exterior Envelopes of Building III, ASHRAE/DOE/BTECC Conference. 1985.
 Straube, J.F. Moisture in buildings. ASHRAE journal. 2002, 44(1)
 Steiger, R.; Hurd M. Lightweight insulating concrete for floors and roof decks. Concrete Construction.
 Hodicky, K.; Sopal G.; Rizkalla S.; Hulin T.; Stang H. Experimental and numerical investigation of
the FRP shear mechanism for concrete sandwich panels. J Compos Constr. 2014, 19(5)
 Kazem, H.; Bunn W.G.; Seliem H.M.; Rizkalla S.H.; Gleich H. Durability and long term behavior of
FRP/foam shear transfer mechanism for concrete sandwich panels. Constr Build Mater. 2015, 98
 Mousa, M.A.; Uddin N. Experimental and analytical study of carbon fiber-reinforced polymer
(FRP)/autoclaved aerated concrete (AAC) sandwich panels. Eng Struct. 2009, 31(10)
 Tomlinson, D.; Fam A. Flexural behavior of precast concrete sandwich wall panels with basalt FRP
and steel reinforcement. PCI J. 2015.
 Teixeira, N.; Tomlinson D.G.; Fam A. Precast concrete sandwich wall panels with bolted angle connections tested in flexure under simulated wind pressure and suction. PCI J. 2016.
 Huanzhi, J.; Zhengxing G.; Jiabin L. Composite behavior of sandwich panels with W-shaped SGFRP
connectors. KSCE J Civ Eng. 2017
 Jiang, H.; Guo Z.; Liu J.; Liu H. The Shear Behavior of Precast Concrete Sandwich Panels with
W-shaped SGFRP Shear Connectors. KSCE J Civ Eng. 2018
 Choi, K.-B.; Choi W.-C.; Feo L.; Jang S.-J.; Yun H.-D. In-plane shear behavior of insulated precast
concrete sandwich panels reinforced with corrugated GFRP shear connectors. Compos Part B-Eng.
 Kim, J.; You Y.-C. Composite behavior of a novel insulated concrete sandwich wall panel reinforced
with GFRP shear grids: Effects of insulation types. Materials. 2015, 8(3)
 Pantelides, C.P.; Surapaneni R.; Reaveley L.D. Structural performance of hybrid GFRP/steel concrete
sandwich panels. J Compos Constr. 2008, 12(5)
 Woltman, G.; Tomlinson D.; Fam A. Investigation of various GFRP shear connectors for insulated
 Tomlinson, D.; Fam A. Experimental investigation of precast concrete insulated sandwich panels with glass fiber-reinforced polymer shear connectors. ACI Struct J. 2014, 111(3)
 Zhi, Q.; Guo Z. Experimental evaluation of precast concrete sandwich wall panels with steel–glass
fiber–reinforced polymer shear connectors. Adv Struct Eng. 2017, 20(10)
 Naito, C.; Hoemann J.; Beacraft M.; Bewick B. Performance and characterization of shear ties for use
in insulated precast concrete sandwich wall panels. J Struct Eng. 2011, 138(1)
 Lameiras, R.; Barros J.; Azenha M.; Valente I.B. Development of sandwich panels combining fibre
reinforced concrete layers and fibre reinforced polymer connectors. Part II: Evaluation of mechanical behaviour. Compos Struct. 2013, 105
 Vilanova, I.; Baena M.; Torres L.; Barris C. Experimental study of bond-slip of GFRP bars in concrete
under sustained loads. Compos Part B-Eng. 2015, 74
 Corradi, M.; Borri A.; Castori G.; Sisti R. Shear strengthening of wall panels through jacketing with
cement mortar reinforced by GFRP grids. Compos Part B-Eng. 2014, 64
 Ascione, L.; Feo L. Modeling of composite/concrete interface of RC beams strengthened with composite laminates. Compos Part B-Eng. 2000, 31(6-7)
 Salmon, D.C.; Einea A.; Tadros M.K.; Culp T.D. Full scale testing of precast concrete sandwich panels. ACI Struct J. 1997, 94
 Rahman, M.; Jaini Z. The combined finite-discrete element analysis of precast lightweight foamed
concrete sandwich panel (PLFP) under axial load. Proceedings of the International Conference on Advances in Structural. 2013.
 Mohamad, N.; Hassan N. The structural performance of precast lightweight foam concrete sandwich
panel with single and double shear truss connectors subjected to axial load. Advanced Materials Research. Trans Tech Publ; 2013.
 Carbonari, G.; Cavalaro S.; Cansario M.; Aguado A. Experimental and analytical study about the compressive behavior of eps sandwich panels. Materiales de Construcción. 2013, 63(311)
 Gara, F.; Ragni L.; Roia D.; Dezi L. Experimental tests and numerical modelling of wall sandwich
panels. Eng Struct. 2012, 37
 Farah, N.A.A.A. Structural Behaviour of Precast Concrete Sandwich Panels with Openings under
Axial Load; MSc. Report
;Universiti Putra Malaysia, 2002.
 Kang, W.-H.; Kim J. Reliability-based flexural design models for concrete sandwich wall panels with
continuous GFRP shear connectors. Compos Part B-Eng. 2016, 89
 Kim, J.; Choi K.-S. Flexural strength for insulated concrete sandwich wall panel reinforced with glass-fiber-reinforced polymer shear grids: roughness-induced mechanical bonding. Materials Research Innovations. 2015, 19(sup8)
 Sousa, C.F.; Barros J.A.; Azenha M.; Lameiras R.M. Flexural and shear behaviour of precast sandwich
slabs comprising thin walled steel fibre reinforced self-compacting concrete. 7th RILEM International Conference on Self-Compacting Concrete and 1st RILEM International Conference on Rheology and Processing of Construction Materials. RILEM; 2013.
 Mathieson, H.; Fam A. Effect of internal ribs on fatigue performance of sandwich panels with GFRP
skins and polyurethane foam core. Journal of Materials in Civil Engineering. 2013, 27(2)
,A4014005.  Henin, E.; Morcous G.; Tadros M.K. Precast/prestressed concrete sandwich panels for thermally efficient floor/roof applications. Practice Periodical on Structural Design and Construction. 2013,
 Flores-Johnson, E.; Li Q. Structural behaviour of composite sandwich panels with plain and fibre-reinforced foamed concrete cores and corrugated steel faces. Compos Struct. 2012, 94(5)
,1555-1563.  Frankl, B.A.; Lucier G.W.; Hassan T.K.; Rizkalla S.H. Behavior of precast, prestressed concrete
sandwich wall panels reinforced with CFRP shear grid. PCI J. 2011, 56(2)
 Lee, B.-J.; Pessiki S. Experimental evaluation of precast, prestressed concrete, three-wythe sandwich
wall panels. PCI J. 2008, 53(2).
 Benayoune, A.; Samad A.A.; Trikha D.; Ali A.A.; Ellinna S. Flexural behaviour of pre-cast concrete
sandwich composite panel–experimental and theoretical investigations. Constr Build Mater. 2008,
 Lee, B.-J.; Pessiki S. Design and analysis of precast, prestressed concrete, three-wythe sandwich wall panels. PCI J. 2007, 52(4)
 Bush, T.D.; Stine G.L. Flexural behavior of composite precast concrete sandwich panels with continuous truss connectors. PCI J. 1994, 39(2).
 Oh, T.S.; Jang S.J.; Lee K.M.; Yun H.D. Insulation type effect on the direct shear behavior of concrete sandwich panel (csp) with non-shear connectors. Advanced Materials Research. Trans Tech Publ; 2013.
 Cho, K.; Park S.Y.; Kim S.T.; Cho J.-R.; Kim B.-S. Shear connection system and performance evaluation of FRP-concrete composite deck. KSCE J Civ Eng. 2010, 14(6)
 Abdou, A.A.; Budaiwi I.M. Comparison of thermal conductivity measurements of building insulation
materials under various operating temperatures. Journal of Building Physics. 2005, 29(2)
,171-184.  Bolattürk, A. Determination of optimum insulation thickness for building walls with respect to various
fuels and climate zones in Turkey. Applied thermal engineering. 2006, 26(11-12)
,1301-1309.  Ucar, A.; Balo F. Effect of fuel type on the optimum thickness of selected insulation materials for the
four different climatic regions of Turkey. Appl Energ. 2009, 86(5)
 Kossecka, E.; Kosny J. Hot-Box Testing of Building Envelope Assemblies—A Simplified Procedure
for Estimation of Minimum Time of the Test. Journal of Testing and Evaluation. 2008, 36(3)
 Ozel, M. Thermal performance and optimum insulation thickness of building walls with different structure materials. Applied Thermal Engineering. 2011, 31(17-18)
 Ekici, B.B.; Gulten A.A.; Aksoy U.T. A study on the optimum insulation thicknesses of various types
of external walls with respect to different materials, fuels and climate zones in Turkey. Appl Energ.
 Yu, J.; Yang C.; Tian L.; Liao D. A study on optimum insulation thicknesses of external walls in hot
summer and cold winter zone of China. Appl Energ. 2009, 86(11)
 Peng, C.; Wu Z. In situ measuring and evaluating the thermal resistance of building construction. Energ Buildings. 2008, 40(11)
 Al-Sanea, S.A.; Zedan M. Improving thermal performance of building walls by optimizing insulation
layer distribution and thickness for same thermal mass. Appl Energ. 2011, 88(9)
,3113-3124.  Tsilingiris, P. Parametric space distribution effects of wall heat capacity and thermal resistance on the
dynamic thermal behavior of walls and structures. Energ Buildings. 2006, 38(10)
,1200-1211.  Kossecka, E.; Kosny J. Influence of insulation configuration on heating and cooling loads in a
continuously used building. Energ Buildings. 2002, 34(4)
 Zarr, R.; Burch D.; Faison T.; Arnold C. Thermal Resistance Measurements of Well-Insulated and Superinsulated Residential Walls Using a Calibrated Hot Box. Journal of Thermal Insulation. 1987,
 Lee, B.-J.; Pessiki S. Analytical investigation of thermal performance of precast concrete three-wythe sandwich wall panels. PCI J. 2004, 49(4).